- Home
- Documents
*Modelling of Transport Phenomena in Laser Welding of Steels ©tais_paper.pdfآ Modelling of...*

prev

next

out of 7

View

0Download

0

Embed Size (px)

Modelling of Transport Phenomena in Laser Welding of Steels A. Métais*1,2, S. Matteï1, I. Tomashchuk1 and S. Gaied2 1Laboratoire Interdisciplinaire Carnot de Bourgogne (ICB), UMR 6303 CNRS / Université Bourgogne Franche-Comté, 71200 Le Creusot, FRANCE 2ArcelorMittal, route de Saint Leu 60761 Montataire, FRANCE *alexandre.metais@arcelormittal.com

Abstract: Laser Welded Blank solutions enable to reduce vehicles weight and to optimize their crash performances by means of simultaneous tuning of different grades and thicknesses. The present work aims to characterize numerically and experimentally materials mixing during laser welding. For better understanding of materials mixing based on convection-diffusion process in case of full penetrated laser welding, a 3D simulation of fluid flow, heat transfer and mass transfer has been performed to provide fusion zone shape and elements distribution map. The model has been developed basing on steady keyhole approximation and solved in quasi-stationary form in order to reduce computation time. Turbulent flow model was used to calculate velocity field. Fick law for diluted species was integrated to simulate the transport of alloying elements in the weld pool. In parallel, a number of experiments using pure Ni foils as tracers have been performed to obtain mapping of Ni distribution in the melted zone. SEM- EDX analysis of chemical composition has been made to map elements distribution in the melted zone. The results of simulation have been found in good agreement with experimental data.

Keywords: Laser welding, dissimilar materials, thermo-hydraulic, transport species.

1. Introduction

The role of Laser Welded Blanks (LWB) in vehicles design is significantly increasing. Car manufacturers aim to develop more and more lightweight and strong car architectures that meet latest crash and safety requirements. The main benefits for LWB are mass and cost savings. Mass savings are achieved due to the higher strength level combinations. A good understanding of phenomena occurring during laser welding is essential to obtain a good quality of the weld. Partially penetrated dissimilar laser welding process has already been studied by using heat, fluid flow and transport species inside a 3D model of melt pool [1]. The present study is focusing on a full penetrated laser welding process. The aim of present modelling is to carry out mechanism of formation of eddies in the weld pool by using specific tracers. Then, these

results could be used to improve laser weld mixing between dissimilar steels.

2. Experimental setup

Experiments tests were carried out with a Yb:YAG laser, a power of 4 kW and spot size of 600 µm. Pure nickel foils (100 µm thick) were introduced between the welded plates. Figure 1 shows a schematic sketch of laser welding process and nickel layer position. Different offset distances of laser beam from joint line were tested: centred position (weld 1) and 200 µm offset from the middle of Ni foil (weld 2).

" Figure 1 - Welding configuration (weld 2)

Nickel was chosen as tracer material to reveal the mixing process in the melted zone because of its similarity with iron in term of density, thermal conductivity and heat capacity. 100 µm thick foils are enough to ensure good traceability with SEM-EDX analysis. In this study it is supposed that addition of small quantity of Ni in the melted zone does not modify significantly local thermophysical properties.

3. Model description

3.1. Assumptions

A number of assumptions have been made to develop the following tridimensional model with the goal to reduce computation time:

• a steady keyhole with a conical geometry;

• temperature inside the keyhole is a s s u m e d t o b e u n i f o r m " ; Tkeyhole = Tvaporization( )

Excerpt from the Proceedings of the 2015 COMSOL Conference in Grenoble

• top and bottom surfaces of the weld are assumed to be flat;

• heat transfer and fluid flow equations are strongly coupled;

• liquid metal is assumed to be newtonian and incompressible;

• quasi-steady approach is used.

3.2. Geometry and mesh

The keyhole is represented by a cone-shaped geometry. Maximal diameter of the cone (top surface) is equal to the diameter of focused laser spot (600 µm) and minimal diameter (bottom surface) is equal to 500 µm. Thickness of the plate is conserved (1.6 mm). A representative volume of the welded blanks is meshed. Tetrahedral mesh of 60 µm maximal size was additionally refined around the keyhole (Figure 2).

" Figure 2 - Mesh and thermal field

4. Governing equations

4.1. Heat transfer

The energy equation solved with convection term provides temperature field over entire domain

"

where" is the density, " - heat capacity, " - conductivity, " - temperature and " - velocity field.

The melting phase change is taken into account by using equivalent enthalpy method

"

where " is heat capacity function of

temperature, " - melting latent heat and " - gaussian distribution defined as

"

where " is temperature range of 100 K and " - melting point of materials.

Heat losses due to convection and radiation are taken into account throughout a global heat exchange coefficient.

"

4.2. Fluid flow

A Reynolds-Averaged Navier-Stokes k-ω turbulent model has been chosen in order to take into account turbulent mixing caused by eddy diffusivity. The governing equations for mass conservation, momentum and energy transport in steady-state formulation are as follows as they are implemented within the simulation framework.

" !

"

"

"

"

where " is density, " - velocity field, " - pressure, " - dynamic viscosity, " - gravity constant and " , " - turbulent flow parameters.

Due to variation of surface tension coefficient with temperature,

"

Marangoni effects are taken into account on the top and bottom surfaces.

"

where " represents the surface tangent.

Full-penetrated welding produces high velocity jet of gas. In literature a velocity of the metallic vapour gas, named plume, higher than 100 m.s-1 can be found [2]. Shear stress due to the interaction of the plume on the liquid metal can’t be neglected and has been introduced to surfaces as a weak contribution. This phenomenon is still misunderstood and in this model shear stress is a constant chosen by the user. Considering that the flow inside the vapour plume is laminar, the Darcy-Weisback equation gives an order of magnitude for the shear stress between liquid metal and vapour plume.

"

ρCpu ⋅∇T +∇(−k∇T ) = 0

ρ Cp k T u

Cp = Cp * (T )+δ ⋅ Lfusion

Cp * (T )

Lfusion δ

δ = 1 ΔT ⋅ π

⋅e T−Tfusion

ΔT ⎛

⎝ ⎜

⎞

⎠ ⎟

ΔT Tfusion

k ! ∇T ⋅ !n = −hg (T −T0 )

ρ∇⋅(u) = 0

ρ(u ⋅∇)u = ∇⋅ − pI + (µ + µT ) ∇u+ (∇u) T( )⎡⎣ ⎤⎦ − ρg + F Marangoni

ρ(u ⋅∇)k = ∇⋅ µ + µTσ k *( )∇k⎡⎣ ⎤⎦ + pk − β0*ρωk

ρ(u ⋅∇)ω = ∇⋅ µ + µTσω( )∇ω⎡⎣ ⎤⎦ +α ω k pk − ρβ0ω

2

µT = ρ k ω

pk = µT ∇u : ∇u+ (∇u) T( )⎡⎣ ⎤⎦

ρ u p µ g

k ω

γ = γ 0 + dγ dT

⋅(T −Tvap )

F Marangoni = ∂γ ∂T

⋅ ∂T ∂τ

τ

τ = 1 8 f ρV 2

Excerpt from the Proceedings of the 2015 COMSOL Conference in Grenoble

where " for a laminar flow, " - density

of the plume and " - velocity of the plume. For a velocity of 100 m.s-1 a surface shear stress of 50 N.m2 has been calculated. This value is currently used in our numerical models without experimental validation.

The moving solid-liquid interface is modeled through changing the viscosity of the fluid. Dynamic viscosity is temperature dependent: solid is assumed as liquid with viscosity of 100 Pa.s (Figure 3).

" Figure 3 - Dynamic viscosity of a equivalent fluid

4.3. Fick Law for diluted species

To study transport of species in weld pool, Fick law has been used:

"

where " is concentration of element " (here

[Ni]), " - velocity field and " - diffusion coefficient of element i defined as:

"

where " is Boltzmann constant, " -

temperature, " - radius of the diffusive particle " and " - dynamic viscosity of fluid.

The hypothesis that material properties like density, conductivity and heat capacity are independent of species concentration is made.

5. Solving method

Heat transfer, turbulent flow and transport of diluted species problems are solved with COMSOL Multyphysics® 5.1. In segregated resolution, direct PARDISO solvers are used to calculate variables T and [Ni] and iterative GMRES solver is used to calculate fluid flow variables. Use of iterative solver allows reduce RAM memory need.

6. Results and discussion

6.1. Weld shape

In this model geometric dimensions and temperature of the keyhole are adjusted in order to obtain weld shape size in good agreement with experiments. An hourglass weld shape is generally observed for full penetrated laser welds. Numerically, a negative temperature coefficient of surface tension " results in hourglass weld shape. The metal flows from the hig